M a c r o m o l e c u l e s 1990, 23, 2402-2406
Acknowledgment is made to the donors of the Petroleum Research Fund, administered by the American Chemical Society, for support Of this research. We are thankful to E. I. du Pont de Nemours & Co., Inc., for their kind donation of Nafion 117 membranes.
mer Materials: Blends, Ionomers, and Interpenetrating Networks; Utracki, L. A.; Weiss, R. A., Eds.; ACS Symposium Series 395; American Chemical Society: Washington, DC, 1989;
( 5 ) Mauritz. K. A.: Jones, C. K. J . A ~ n lPolvm. . Sci.. in Dress. (6) Yeo, S.C.; Eisenberg, A. J . A p p l Polym."Sci. 1977, 21, 875. ( 7 ) McCrum, N. G. J . Polym. Sei. 1959, 34, 355. (8) Kyu, T,; Eisenberg, A, In Perfluorinated Ionomer Membranes; ACS Symposium Series 180; Eisenberg, A., Yeager, H. L., Eds.; American Chemical Society: Washington, DC, 1982; 13 79. (9) Moore, R. B.; Martin, C. R. Macromolecules 1988,21, 1334. (10) Starkweather. H. W.. Jr. Macromolecules 1982. 15, 320. (11) Mauritz, K. A. J . Macromol. Sci., Reu. Mac'romol. Chem. Phys. 1988, C28 (l), 65. (12) Gierke. T. D.: Munn. G. E.: Wilson. F. C. In Perfluorinated lonomer Membranes, ACS Symposium Series 1801Eisenberg, A., Yeager, H. L., Eds.; American Chemical Society: Washington, DC, 1982; p 195.
p 401. (3) Mauritz, K. A.; Warren, R. M. Macromolecules 1989,22,1730. (4) Mauritz, K. A.; Stefanithis, I. D. Macromolecules, in press.
Registry No. TEOS, 78-10-4; Nafion 117, 66796-30-3;silicon oxide, 7631-86-9.
References a n d Notes (1) Nafion is a registered trademark of E. I. du Pont de Nemours & Co., Inc. ( 2 ) Mauritz, K. A.; Storey, R. F.; Jones, C. K. In Multiphase Poly-
Evidence for Molecular Cr3+ Cross-Links in Cr3+/Polyacrylamide Gels Giovanni Burrafato, Stefan0 Carminati, Fabrizio Bonaccorsi, a n d Thomas P. Lockhart' Eniricerche S.p.A., via M a r i t a n o 26, 20097 San Donato Milanese, Italy. Received July IO, 1989; Revised Manuscript Received October 26, 1989
ABSTRACT The gelation of buffered aqueous solutions of Cr3+ and polyacrylamide having a low degree of hydrolysis (0.7% and 10%) has been investigated over a wide range of pH. It has been found that gelation occurs between pH 2.3 and 6.7 and that the time of gelation increases dramatically at low pH. An inverse correlation between Cr(OH),(H,O), colloid formation (revealed by solution turbidity) and the pH range of gelation indicates that discrete, soluble (monomeric or oligomeric) rather than colloidal forms of Cr3+ are responsible for the cross-linking. The occurrence of gelation in the pH interval 6.0-6.7, where only a small amount of the Cr3+ would be soluble in a simple aqueous solution, has been attributed tentatively to Cr3+ complexation by the polymer. Cr3+ solubility experiments at pH 6.6 in solutions containing model, monomeric carboxylate compounds lend support for this hypothesis. Aqueous polymer gels composed of high molecular weight, partially hydrolyzed polyacrylamide (or other synthetic or biopolymers) cross-linked by Cr3+ or A13+ are of interest for use in augmenting the petroleum recovery from mature reservoirs."' So-called secondary oil recovery typically involves the continuous injection of water into a reservoir from a subset of the existing wells. The injected water physically displaces to the other wells a significant portion of the mobile oil with which it comes into contact. A major limitation to petroleum recovery by this method arises from the fact that most reservoirs are compositionally heterogenous and that the injected water floods preferentially the strata of highest permeability. A promising but still experimental reservoir treatment involves the occlusion of the higher permeability strata, after preliminary water flooding, with polymer gels which are formed within the reservoir from aqueous polymer/cross-linker solutions. Water injected subsequently is thereby diverted to lower permeability zones, and the mobile oil contained therein can be recovered. Among the various enhanced oil recovery techniques proposed and field-tested during the past 15 years, reservoir profile modification with aqueous polymer gels remains one of the few economically promising strategies in the present period of low-priced petroleum. Several chemical impediments remain that prevent the 0024-9297/90/2223-2402$02.50/0
full realization of the gel profile modification strategy. These include instability of the polymeric gels a t high temperature, limited control over and understanding of the kinetics of gelation, and lack of satisfactory mathematical models which permit the controlled placement of the gels within the reservoir. A more detailed understanding of the structure and chemistry of the metal ion cross-links in these gels should aid in the rational design of aqueous gels having improved performance characteristics. Both colloidal and discrete molecular cross-link structures have been suggested3s4 for aqueous polymer gels cross-linked with Cr3+ (Figure 1). The distinction between the two types of cross-links is of great practical importance, since the development of accurate kinetic models of gelation and reliable predictions of gel stability under varying conditions depend on a knowledge of the structure and chemistry of the cross-link. In the present paper, we describe conceptually simple experiments on Cr3+/ polyacrylamide (PAAm) gels which provide clear evidence for a molecular Cr3+ cross-link structure. Results a n d Discussion The cross-linking chemistry of Cr3+/PAAm gels depends on the complex aqueous solution chemistry of Cr3+,which has been elucidated in remarkable detail over the past 0 1990 American Chemical Society
Macromolecules, Vol. 23, No. 8,I990
Molecular Cross-Links in Cr3+/Polyacrylamide Gels 2403 Table I pH Dependence of Cr3+/PAAmGel Formation at 25 Unbuffered Solutions'
4.0 5.1 6.1 7.0 8.1 10.1
Figure 1. Representation of colloidal (upper)and discrete molecular (lower) Cr3+ cross-links. One possible form (dimeric in Cr3+)has been represented for the latter.
Figure 2. Aqueous solution chemistry of Cr3+ (see refs 5-8).
80 years."' The main features of this chemistry are illustrated in Figure 2. The predominant species a t low pH is Cr(H20)z+,but equilibria with monomeric Cr3+mono-, di-, and trihydroxides are established rapidly a t higher pH. The trihydroxide, Cr(0H) (H20),, is extremely insoluble in water ( K , = 10-30.3)sb3andprecipitates a t moderate pH. The sofuble mono- and dihydroxides convert to dimeric and higher oligomeric species with rate constants that depend on temperature and pH6 but are similar in magnitude to the rate of gelation of Cr3+/PAAm solutions. I t is apparent from this description that both molecular (monomeric or oligomeric) and colloidal (i.e., Cr(OH),(H,O),) forms of Cr3+ may be available for crosslinking with PAAm over an interval of solution pH which depends on temperature and the Cr3+ concentration. In order to evaluate the possible role of molecular and colloidal forms of Cr3+ in the cross-linking of polyacrylamide gels, we have carried out a systematic investigation of the gelation of Cr3+/PAAm solutions (9.6 X M (50 ppm) in Cr3+ and 8000 ppm in PAAm 0.7% hydrolyzed) as a function of pH. In preliminary experiments, Cr3+/PAAm solutions were prepared having initial pH values from pH 2.0 to 10.1. The gelation results are summarized in Table I along with the estimatedsb solubility of Cr3+ in water at each pH. Gels formed with widely varying rates in the pH range 3.0-7.0 a t 25 OC. The presence of colloidal Cr3+ in the solutions a t pH 7.0 and above was indicated by their turbidity. The correlation of gelation with pH requires that the
pH at 60 days
2.5 6.2 6.9 7.4 7.9
gel time, days
estimated soluble Cr3+,b %
100 100 100 14 0.5